2. • Introduction
• Gypsom types
• Requirements of dental cast materials
• Manipulation and setting characteristics
• Setting Time
• Control expantion
• Properties of setting
• Advantages and disadvantages
• Infection control
• Gypsum is a naturally occurring,
white powdery mineral with the
chemical name calcium sulphate
• Gypsum products used in
dentistry are based on calcium
(CaSO42)2·H2O. Their main uses
are for casts or models, dies .
4. • models and dies which should
be accurate replicas of the
patient’s hard and soft tissues.
• model is a replica of several
teeth and their associated soft
tissues or, alternatively, to an
• die is a replica of a single
5. • The morphology of the hard and soft
tissues is recorded in an impression
and models and dies are prepared
10. 1. dimensional accuracy
2. adequate mechani-cal properties
3. The material should be ﬂuid at the time it is
poured into the impression so that ﬁne detail
can be recorded
4. A low contact angle between the model and
impression materials would
help to minimize the presence
of surface voids on the set
model by encouraging surface
11. 5. The set material should be strong to resist
accidental fracture and hard enough to
resist abrasion during the carving of a wax
6. The material should be compatible with all
the other materials with which it comes
12. • Gypsum products used in dentistry are formed
by driving off part of the water of crystallization
from gypsum to form calcium sulphate
• Gypsum → Gypsum product + water
• 2CaSO4·2H2O → (CaSO4)2·H2O + 3H2O
13. • Dental plaster (plaster of
Paris): Dental plaster is
indistinguishable from the
white plaster used in
orthopaedics for stabilizing
fractured limbs during bone
healing. Plaster is produced
by a process known as
14. • Gypsum is heated to a temperature of about
120ºC in order to drive off part of the water of
crystallization. This produces irregular, porous
particles which are sometimes referred to as
Dental plaster =>
kettle ) at 120ºC β-
16. • Overheating the gypsum may cause further
loss of water to form calcium sulphate
• underheating produces a signiﬁcant
concentration of residual dihydrate. The
presence of both components has a marked
inﬂuence upon the setting characteristics of
the resultant plaster.
17. • Dental stone => gypsom
+ steam & pressure at
(type 3 gypsum)
19. • Dental stone: Dental stones may be produced
byone of two methods. If gypsum is heated to
about125ºC under steam pressure in an
autoclave a more regular and less porous
hemihydrate is formed This is sometimes
referred to as an α-hemihydrate. Alternatively,
gypsum may be boiled in a solution of a salt
such as CaCl2. This gives a material similar to
that produced by autoclaving but with even
less porosity. Manufacturers normally add
small quantities of a dye to dental stones in
order that they may be differentiated from
dental plaster, which is white.
22. Plaster and stone powders are mixed
with water to produce a workable mix.
Hydration of the hemihydrate then
occurs producing the gypsum model or
23. • Considerable quantities of air may be
incorporated during mixing and this may lead to
porosity within the set material. Air porosity may
be reduced either by vibrating the mix of plaster
or stone in order to bring air bubbles to the
surface or by mixing the material mechanically
under vacuum, or both.
24. • For hand mixing a clean, scratch free
rubber or plastic bowl having a top
diameter of about 130 mm is
• Should be clean because the
gypsum residues in the mixing bowl
can noticeably alter the working and
A stiff spatula with a round-edged
blade of around 20–25 mm width
and 100 mm length is used.
25. • the amount of water needed is
added to a moist bowl and the
powder added slowly to the water
over about 10 seconds.
• mixing/spatulation carried out for
around 60 seconds using a circular
or figure of eight motion.
• After the material has been mixed
and used, the mixing bowl should
be thoroughly cleaned before the
next mix is performed.
26. • The crystals of dihydrate are spherulitic in nature
and grow from speciﬁc sites called nuclei of
crystallization. These may be small particles of
impurity, such as unconverted gypsum crystals,
within the hemihydrate powder. If a thin mix of
material is used, containing more water, the
formation of the super-saturated solution of
dihydrate which is a precursor to crystallization is
delayed and the centers of nucleation are more
widely dispersed by the dilution effect. The set
plaster is therefore less dense with greater
spaces between crystals leading to a signiﬁcant
reduction in strength.
27. • The material should be used as soon as
possible after mixing since its viscosity
increases to the stage where the material
is unworkable within a few minutes.
• The setting reaction is exothermic
28. • The setting characteristics of gypsum
products can be affected
1.by the presence of unconverted dihydrate
2.by the presence of anhydrite
3.the age of the material
4. the storage conditions
• Small quantities of unconverted dihydrate act
as centres of nucleation as mentioned earlier.
• Anhydrite reacts very rapidly with water
producing a marked acceleration in setting.
29. • Another physical change which accompanies
setting is a small expansion caused by the
30. • The maximum rate of expansion occurs at the
time when the temperature is increasing most
rapidly. The expansion is, in fact, only
apparent since the set material contains a
considerable volume of porosity. If the
material is placed in water at the initial set
stage, considerably more expansion occurs
during setting. This increased expansion is
called hygroscopic expansion
33. 2. W/P ratio
• Increasing the W/P ratio retards setting by
decreasing the concentration of crystallization
34. 3. mixing time
• Increasing mixing time has the opposite
effect. This accelerates setting by breaking up
dihydrate crystals during the early stages of
setting,thus producing more nuclei on which
crystallization can be initiated.
36. • A higher concentration of nucleating agent, pro-
duced by ageing or from unconverted calcium
sulphate dihydrate, results in more rapid
crystallization. Also, the manufacturers may add
chemical accelerators or retarders to dental
• Potassium sulphate is a commonly used
accelerator which is thought to act by increasing
the solubility of the hemihydrate. Borax is the
most widely used retarder, although the
mechanism by which it works is not clear.
37. • In order to produce an accurate model or die it is
necessary to maintain the setting expansion at as
low a value as possible.
• Accelerators or retarders which are added by
manufacturers to dental stones in order to
control the setting time also have the effect of
reducing the setting expansion and are
sometimes referred to as antiexpansion agents.
• Alterations in W/P ratio and mixing time have
only a minimal effect on setting expansion.
39. • The strength of gypsum depends, primarily,
1. porosity of the set material
2. the time for which the material is allowed to
dry out after setting.
• The porosity, and hence the strength, is
proportional to the W/P ratio
• Since stone is always mixed at a lower W/P
ratio than plaster it is less porous and
consequently much stronger and harder.
41. • Although a gypsum model or die may appear
completely set within a relatively short period its
strength increases signiﬁcantly if it is allowed to
stand for a few hours.
• Greatest surface hardness
reach its dry strength , it
should be allowed to set for
one or two hours preferable
for night before laboratory
occurs when product
42. • gypsum is a very brittle material.
• very low value of ﬂexural strength of plaster
• Stone is less fragile but must be treated with
care if fracture is to be avoided. It is relatively
rigid but has a poor impact strength and is
likely to fracture if dropped.
• Attempts to improve the mechanical
properties have involved
1.the impregnation by a polymer such as acrylic
2.lower W/P ratio.
43. • The dimensional stability
of gypsum is good.
following setting, further
changes in dimensions are
immeasurable and the
materials are sufficiently
rigid to resist deformations
when work is being carried
out upon them.
44. • Set plaster is slightly soluble in water.
Solubility increases with the temperature of the
water and if hot water is poured over the
surface of a plaster cast, as happens during the
boiling out of a denture mould, a portion of the
surface layer becomes dissolved leaving the
surface roughened. Frequent washing of the
surface with hot water should therefore be
47. • When strength, hardness and accuracy are
required dental stones are normally used in
preference to dental plaster.
• The stone materials are less likely to be damaged
during the laying down and carving of a wax
pattern and give optimal dimensional accuracy.
• Thus, these materials are used when any work is
to be carried out on the model or die as would be
the case when constructing a denture on a model
or a cast alloy crown on a die.
• When mechanical properties and accuracy are
not of primary importance the cheaper dental
plaster is used. Thus, plaster is often used for
mounting stone models onto articulators and
sometimes for preparing study models
48. •Type I : Impression material rarely used
Non-elastic impression material
• Type II Model of plaster used for
2.articulation of stone cast
3. Art portion working cast
4. Flasking procedure for acrylic
49. • Type III Dental stone used for
1.full or partial denture model
3. Flasking procedure for
• Type IV Dental stone used for
1.fabricating wax patterns of
cast restoration (crown and
51. • Gypsum model and die materials have the
2.easy to use.
3.The accuracy and dimensional stability are good
4. reproduce ﬁne detail from the impression
1. The mechanical properties are not ideal
2. the brittle nature of gypsum occasionally leads to
fracture – particularly through the teeth, which
form the weakest part of any model.
52. • Problems occasionally arise when gypsumproducts
are used in conjunction with alginate impression.
• The surface of the model may remain relatively soft
due to an apparent retarding effect which
hydrocolloids have on the setting of gypsum
products. It is not certain whether the retarding
effect is due to borax in the hydrocolloid or to the
absorption of hydrocolloid onto the gypsum crystals
which act as nuclei of crystallization.
• Despite these observations it cannot be said that
gypsum products are incompatible with alginate
impression materials since problems arise very
53. • Alternative materials for the production of
models and dies exist but are hardly ever
• These include various resins, cements and
• The alternatives may be stronger but are
generally less stable, difﬁcult to use and more
54. • Another treatment which has been suggested
for improving the durability of gypsum is to
partly saturate the set material in a
polymerizable monomer such as
methylmethacrylate or styrene.
• Polymerisation of the monomer produces a
polymer phase which increases its strength and
• Despite these apparent advantages these
techniques are rarely used in practice.
56. • Applied Dental Material
by John F McCabe &Angus
Chapter 3 (pages from41-48)
57. • Done by :
Weam Mahmoud Faroun
Third Year Dental Student
• Under supervision :
DR. Mudar Kamal
• Course :
• Date :
Notas do Editor
For example, the set model should easily be removed from the impression without damage to its surface and fracture of teeth. It should give a
good colour contrast with the various waxes which are often used to produce wax patterns.
This produces irregular, porous particles which are sometimes referred to as β-hemihydrate particles.
يعني انه قوة الجبسوم بروداكت بتزيد ازا تركتها فترة بعد ال ستنج
The increase in strength is a function of the loss of excess water by evaporation. It is thought that evaporation of water causes a precipitation of any dissolved dihydrate and that this effectively cements together the crystals of gypsum formed during setting